Structure of the high-temperature phase of caesium nitrate – the importance of high-resolution data
Fábry, Jan; Kučeráková, Monika; Dušek, Michal; Buixaderas, Elena; Hlinka, Jiří; Acta Crystallographica Section B 78 (2022) –; doi:10.1107/S2052520622001135

data_2108929
_publ_section_title
;
 Structure of the high-temperature phase of caesium nitrate -- the
 importance of high-resolution data
;
_journal_coeditor_code           YV5002SUP1
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first
;
;
_journal_paper_doi               10.1107/S2052520622001135
_journal_volume                  78
_journal_year                    2022
_chemical_formula_moiety         'Cs N O3'
_chemical_formula_sum            'Cs N O3'
_chemical_formula_weight         194.9
_chemical_name_common            'caesium nitrate'
_chemical_name_systematic
; 
caesium nitrate
;
_space_group_IT_number           221
_space_group_name_Hall           '-P 4 2 3'
_space_group_name_H-M_alt        'P m -3 m'
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90.000(12)
_cell_angle_beta                 90.000(12)
_cell_angle_gamma                90.000(12)
_cell_formula_units_Z            1
_cell_length_a                   4.5226(6)
_cell_length_b                   4.5226(6)
_cell_length_c                   4.5226(6)
_cell_measurement_reflns_used    1623
_cell_measurement_temperature    440(5)
_cell_measurement_theta_max      44.0900
_cell_measurement_theta_min      4.4830
_cell_volume                     92.50(2)
_computing_cell_refinement       'CrysAlis PRO (Rigaku OD, 2018)'
_computing_data_collection
;
CrysAlis PRO (Rigaku OD, 2018)
;
_computing_data_reduction        'CrysAlis PRO (Rigaku OD, 2018)'
_computing_molecular_graphics
;
Diamond 3.2e (Brandenburg, 2015);
Mercury 4.0 (Macrae et al., 2020)
;
_computing_publication_material  <i>JANA</i>2006
_computing_structure_refinement
;
<i>JANA</i>2006 (Pet\<r\'i\<cek <i>et al.</i>, 2014)
;
_computing_structure_solution
;
<i>SUPERFLIP</i> (Palatinus & Chapuis, 2007)
;
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      440(5)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 5.1783
_diffrn_detector_type            AtlasS2
_diffrn_measured_fraction_theta_max 1.0000
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, AtlasS2, Gemini ultra'
_diffrn_measurement_method       'Oxford Diffraction CCD'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0372
_diffrn_reflns_av_unetI/netI     0.0046
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            4035
_diffrn_reflns_theta_full        45.01
_diffrn_reflns_theta_max         45.01
_diffrn_reflns_theta_min         4.51
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    9.834
_exptl_absorpt_correction_T_max  0.46400
_exptl_absorpt_correction_T_min  0.347
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.41.93a (Rigaku Oxford Diffraction, 2020)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.4988
_exptl_crystal_description       prism
_exptl_crystal_F_000             86
_exptl_crystal_size_max          0.391
_exptl_crystal_size_mid          0.093
_exptl_crystal_size_min          0.078
_refine_diff_density_max         0.64
_refine_diff_density_min         -0.38
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    2.18
_refine_ls_goodness_of_fit_ref   1.87
_refine_ls_number_constraints    0
_refine_ls_number_parameters     14
_refine_ls_number_reflns         109
_refine_ls_number_restraints     2
_refine_ls_R_factor_all          0.0220
_refine_ls_R_factor_gt           0.0144
_refine_ls_shift/su_max          0.0484
_refine_ls_shift/su_mean         0.0275
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0004I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0543
_refine_ls_wR_factor_ref         0.0588
_reflns_number_gt                74
_reflns_number_total             109
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            yv5002sup1.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/IUCr/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_database_code               2108929
_cod_database_fobs_code 2108929